| ||Format||Pages||Price|| |
|7||$50.00||  ADD TO CART|
|Hardcopy (shipping and handling)||7||$50.00||  ADD TO CART|
|Standard + Redline PDF Bundle||14||$60.00||  ADD TO CART|
Significance and Use
4.1 This practice provides standardized requirements for making, curing, protecting, and transporting concrete test specimens under field conditions.
4.2 If the specimens are made and standard cured, as stipulated herein, the resulting strength test data when the specimens are tested are able to be used for the following purposes:
4.2.1 Acceptance testing for specified strength,
4.2.2 Checking adequacy of mixture proportions for strength, and
4.2.3 Quality control.
4.3 If the specimens are made and field cured, as stipulated herein, the resulting strength test data when the specimens are tested are able to be used for the following purposes:
4.3.1 Determination of whether a structure is capable of being put in service,
4.3.2 Comparison with test results of standard cured specimens or with test results from various in-place test methods,
4.3.3 Adequacy of curing and protection of concrete in the structure, or
4.3.4 Form or shoring removal time requirements.
1.1 This practice covers procedures for making and curing cylinder and beam specimens from representative samples of fresh concrete for a construction project.
1.2 The concrete used to make the molded specimens shall be sampled after all on-site adjustments have been made to the mixture proportions, including the addition of mix water and admixtures. This practice is not intended for making specimens from concrete not having measurable slump or requiring other sizes or shapes of specimens.
1.3 1.3 This practice is not applicable to lightweight insulating concrete or controlled low strength material (CLSM).
Note 1: Test Method covers the preparation of specimens and the determination of the compressive strength of lightweight insulating concrete. Test Method covers procedures for the preparation, curing, transporting and testing of cylindrical test specimens of CLSM.
1.4 The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use. (Warning—Fresh hydraulic cementitious mixtures are caustic and may cause chemical burns to exposed skin and tissue upon prolonged exposure.)
1.6 The text of this standard references notes which provide explanatory material. These notes shall not be considered as requirements of the standard.
1.7 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C125 Terminology Relating to Concrete and Concrete Aggregates
C138/C138M Test Method for Density (Unit Weight), Yield, and Air Content (Gravimetric) of Concrete
C143/C143M Test Method for Slump of Hydraulic-Cement Concrete
C172/C172M Practice for Sampling Freshly Mixed Concrete
C173/C173M Test Method for Air Content of Freshly Mixed Concrete by the Volumetric Method
C231/C231M Test Method for Air Content of Freshly Mixed Concrete by the Pressure Method
C330/C330M Specification for Lightweight Aggregates for Structural Concrete
C403/C403M Test Method for Time of Setting of Concrete Mixtures by Penetration Resistance
C470/C470M Specification for Molds for Forming Concrete Test Cylinders Vertically
C495/C495M Test Method for Compressive Strength of Lightweight Insulating Concrete
C511 Specification for Mixing Rooms, Moist Cabinets, Moist Rooms, and Water Storage Tanks Used in the Testing of Hydraulic Cements and Concretes
C617/C617M Practice for Capping Cylindrical Concrete Specimens
C1064/C1064M Test Method for Temperature of Freshly Mixed Hydraulic-Cement Concrete
C1077 Practice for Agencies Testing Concrete and Concrete Aggregates for Use in Construction and Criteria for Testing Agency Evaluation
C1611/C1611M Test Method for Slump Flow of Self-Consolidating Concrete
C1758/C1758M Practice for Fabricating Test Specimens with Self-Consolidating Concrete
D4832 Test Method for Preparation and Testing of Controlled Low Strength Material (CLSM) Test Cylinders
American Concrete Institute Publication309R Guide for Consolidation of Concrete
ICS Number Code 91.100.30 (Concrete and concrete products)
UNSPSC Code 30111500(Concrete and mortars)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM C31 / C31M-19a, Standard Practice for Making and Curing Concrete Test Specimens in the Field, ASTM International, West Conshohocken, PA, 2019, www.astm.orgBack to Top